Abstract
Using the van der Waals density functional with C09 exchange (vdWDFC09), which has been applied to describing a wide range of dispersionbound systems, we explore the physical properties of prototypical ABO_{3} bulk ferroelectric oxides. Surprisingly, vdWDFC09 provides a superior description of experimental values for lattice constants, polarization and bulk moduli, exhibiting similar accuracy to the modified PerdewBurkeErzenhoff functional which was designed specifically for bulk solids (PBEsol). The relative performance of vdWDFC09 is strongly linked to the form of the exchange enhancement factor which, like PBEsol, tends to behave like the gradient expansion approximation for small reduced gradients. These results suggest the generalpurpose nature of the class of vdWDF functionals, with particular consequences for predicting material functionality across dense and sparse matter regimes.
Similar content being viewed by others
Introduction
ABO_{3} perovskite oxides, such as PbTiO_{3} and Pb(Zr, Ti)O_{3}, are an important family of multifunctional compounds due to their high dielectric and piezoelectric responses^{1,2,3}. These materials are attractive for numerous technological applications such as electronics, catalysis, superconductors, and electromechanical energy conversion^{4,5}. Recently, major efforts have been invested in designing new leadfree piezoelectric oxides in order to minimize environmental damage^{6,7,8,9,10}. Firstprinciples methods based on density functional theory (DFT) have been routinely used to explore the ferroelectric phase transition of transition metal oxides at the atomistic level. A key challenge is the fact that complex behavior such as orderdisorder transitions and domain wall motion typically require a large number of atoms in order to adequately simulate this behavior. Thus, some of the most common tactics for efficiently studying ferroelectric phase transitions include: (1) Monte Carlo simulations employing DFT parameterized effective Hamiltonians^{11,12,13,14,15,16,17} or (2) molecular dynamic simulations with atomistic potentials, such as the shellmodel^{18,19,20} or bondvalence^{21,22,23} approach. While the above methods correctly reproduce the overall sequence of phase transitions for various perovskite oxides, the values of transition temperatures were generally underestimated relative to the experiments^{11,12,24}. Such discrepancies in transition temperatures is likely caused by a combination of issues including an insufficient description of thermal expansion effects, failure to capture the important cooperative effects of ferroelectric distortions, and/or the error associated with the choice of DFT exchangecorrelation functional^{25,26,27,28,29}.
It is known that the practical error of DFT is closely related to its treatment of exchange and correlation effects. The binding energy between atoms tends to be overestimated by the local density approximation (LDA), resulting in an underestimation of optimized lattice parameters, particularly in perovskite oxides^{30,31}. In contrast, the generalized gradient approximation (GGA) overcorrects the LDA errors, resulting in an overestimation of lattice parameters. Due to the strong volume dependence of structural instabilities in ferroelectric materials^{31,32,33,34,35,36,37}, even modest errors in the values of their lattice parameters may sometimes lead to sizeable inaccuracies in predicting their functional properties with DFT. To overcome this issue, numerous approaches have been proposed to improve the exchange and correlation part of the density functional. Wu and Cohen modified the GGA functional (WCGGA) by tuning the exchange enhancement factor of PerdewBurkeErzenhoff (PBE), which resulted in a better description of ferroelectric PbTiO_{3} and BaTiO_{3} phases compared to GGA and metaGGA^{38}. A similar approach was also adopted by Perdew and coworkers for their modified PBE for solids (PBEsol) functional, which gives predicted lattice parameters in good agreement with experimental values for various materials^{39}. Hybrid exchangecorrelation functionals, such as HSE and B1WC, have also been developed to provide accurate descriptions of structural and electronic structures of ferroelectric oxides^{40,41}. More recently, the class of van der Waals density functionals (vdWDF), which account for longrange dispersion interactions, has shown remarkable success in representing not only dispersionbound, but also denselypacked systems, including ferroelectric bulk oxides and metals^{42,43,44,45,46,47,48,49,50,51,52,53,54}.
In this paper, we study how the choice of exchangecorrelation functionals affects the prediction of the structural and ferroelectric properties of prototypical PbTiO_{3} (PTO), BaTiO_{3} (BTO), and KNbO_{3} (KNO) perovskites. As expected, LDA underestimates both the lattice parameters and spontaneous polarizations, while PBE overestimates them. In contrast, we observed the opposite trend when evaluating the bulk modulus due to the inverse relationship between total energy and optimized volume. Overall, vdWDF with C09 exchange (vdWDFC09), followed by PBEsol, provides the best agreement with the experimental values, demonstrating its utility as a generalpurpose functional for studying ferroelectric perovskite oxides. Additional analyses of the doublewell potential surfaces and phase transition temperatures clearly confirm that the choice of the exchange and correlation functional may significantly impact the values of predicted ferroelectric properties of perovskite oxides. Recent studies on the application of a similar functional, vdWDFcx, to various systems, ranging from the ferroelectric response in PTO to the adsorption of small molecules, further supports the robustness of such vdWDFtype functionals^{52,53,55}. The overall trends in the performance of different functionals can be strongly correlated with the behavior of the exchange enhancement factor in the small reduced gradient region.
Computational Details
All DFT calculations were performed using the planewavebased Quantum Espresso software package^{56}. The energy cutoff for the planewave basis set was 50 Ry (200 Ry for the charge density cutoff), along with ultrasoft pseudopotentials^{57} (scalarrelativistic for A and Bsite cations and nonrelativistic for O) to represent the electronion interaction. This cutoff criterion has also been employed in highthroughput DFT calculations using the ultrasoft pseudopotential library proposed by Garrity, Bennett, Rabe, and Vanderbilt^{58}. Ba (5s, 5p, 5d, 6s, 6p), K (3s, 3p, 4s, 4p), Nb (4s, 4p, 4d, 5s, 5p), Pb (5d, 6s, 6p), Ti (3s, 3p, 3d, 4s), and O (2s, 2p) were considered as valence orbitals. A MonkhorstPack kpoint mesh of 4 × 4 × 4 was determined to be sufficient for sampling the Brillouin zone. The quasiNewton BFGS algorithm was used to optimize the bulk geometry with a force convergence criterion of 3.0 × 10^{−4} Ry/Bohr. To compare the effects of various exchangeandcorrelation parameterizations on the structural and ferroelectric properties of perovskite oxides, we considered four types of functionals: LDA^{59}, PBE^{60}, PBEsol^{39}, and vdWDF^{43,44} with C09 exchange (vdWDFC09)^{47}.
A 2 × 2 × 2 unit cell, consisting of 40 atoms, was first constructed to represent the centrosymmetric bulk structure of cubic PTO, BTO, and KNO perovskites. Subsequent displacements of Bsite cations along [001], [011], and [111] directions were then induced to create tetragonal, orthorhombic, and rhombohedral phases, respectively. The detailed structural information of each crystal phase for PTO, BTO, and KNO can be found in Table S1 of Supplementary Information. In all cases, the cell parameters were relaxed together with the ionic coordinates, using a stress convergence criterion of 0.5 kbar. The Berry phase approach^{61} was applied to calculate spontaneous polarizations, P, from the optimized bulk geometries. The bulk modulus, B, of each crystal phase was evaluated using the BirchMurnaghan^{62} equation of state:
where E_{o} and V_{o} are the total energy and optimized volume of each phase, respectively. Thus, B and its first derivative, B′, can be computed by fitting the above equation with DFT energies and volumes near the energy minimum.
Results and Discussion
Influence of exchangecorrelation functionals on structural properties
Figure 1 shows the percent error of DFT lattice parameters for PTO, BTO and KNO in different crystal phases relative to the experimental values (the magnitudes of the lattice parameters are presented in Table 1). As expected, LDA always underestimates the lattice parameters, while PBE overestimates them. In particular, there is a significant overestimation of the c lattice parameter (as large as ~15% deviation) in the tetragonal phase when using the latter. In contrast, PBEsol and vdWDFC09 predicted lattice parameters close to the experimental values (less than ~3% deviation).
As mentioned above, some of the most responsive piezoelectrics are perovskite oxides. Piezoelectricity is closely related to the following properties: the compressibility of the materials and the magnitude and orientation of polarization^{63,64,65}. In this regard, correctly estimating the spontaneous polarization and elastic properties is the key to understanding phase transition temperatures and electromechanical coupling. Thus, it is an important task to study the exchange and correlation effects on the prediction of these properties for the accurate measurement of piezoelectric responses in perovskites. The bulk modulus and spontaneous polarizations of PTO, BTO, and KNO in different crystal phases were computed and compared to experiment (Table 1). Figure 2 depicts the ratio of the DFT spontaneous polarization (P_{DFT}) relative to the experimental value (P_{Expt}) as a function of the ratio of the DFT bulk modulus (B_{DFT}) relative to experiment (B_{Expt}). Again, using LDA and PBE leads to the under and overestimation of spontaneous polarizations, respectively. The opposite trend was observed for the bulk modulus, generally with larger errors compared to the lattice parameters. The trend in bulk moduli is a direct consequence of the inverse dependence of total energy on optimized volume as shown in Equation (1). In other words, overestimations in volume are translated to underestimations in bulk moduli^{66}. Overall, we found that vdWDFC09 produces the best agreement with experiments when predicting the structural properties of perovskite oxides, while PBEsol yields a slightly lower accuracy in property evaluations compared to the former. In fact, similar performance was also seen with vdWDFcx when predicting the material properties for cubic and tetragonal phase of PTO^{52}. Thus, vdWDFC09 and PBEsol functionals should be suitable for further studies on the phase transitions of ferroelectric oxides.
A closer look at the exchange enhancement factor (F_{x}(s)), which is a function of the reduced density gradient (s = ∇ρ/ρ), shows a clear difference in the overall trends with respect to the form of the exchange functionals, as displayed in Fig. 3. For a standard GGA, the exchange energy, E_{x}(s), can be written as:
where is the exchange energy per particle in a uniform gas with K_{F} = 3π^{2}n. For s < 2, F_{x}(s) of vdWDFC09 matches PBEsol, which tends to the form of the gradient expansion approximation (GEA)^{67}; where F_x(s) = 1 + \mu s_{2} with \mu=0.0864. On the other hand, F_{x}(s) of PBE significantly deviates from the GEA in the small s region. For large s, vdWDFC09 recovers the behavior of the revised PBE (revPBE)^{68} exchange, while PBEsol asymptotes to the PBE limit. Since reducing F_{x}(s) for small s values leads to a decrease in shortrange repulsion^{39,47}, the treatment of F_{x}(s), and thus, shortrange repulsion by PBE leads to the overestimation of structural properties, while the opposite holds true for LDA (whose F_{x}(s) = 1). F_{x}(s) of PBEsol and vdWDFC09 sits between LDA and PBE and behaves similarly in the small s region, providing a more suitable prediction in structural properties compared to both LDA and PBE.
Influence of exchangecorrelation functionals on ferroelectric properties
It is generally thought that the magnitude of the ferroelectric double well potential depth scales with the magnitude of the polarization. Changes in the predictions of ferroelectric well depths, consequently, may have large effects on predictions of ferroelectric phase transitions as well as responses to the application of an external electric field. The double well potential for the cubictotetragonal transition can be expressed as a function of DFTderived spontaneous polarizations based on the Landau theory (without considering strain couplings)^{69}:
where ΔE is the total energy relative to the saddle point and P is the spontaneous polarization from DFT calculations. At the ferroelectric minimum, Equation (3) can be rearranged to find the value of constants: and . Greater potential well depths are expected for PTO, due to the presence of Pb lone pairs which results in a stronger hybridization between Pb 6s and O 2p orbitals resulting in larger polarizations in PTO as compared to BTO and KNO^{33}. More importantly, we observed that the potential well depth increases by the following order of functionals regardless of the material: LDA ≤ vdWDFC09 < PBEsol < PBE, as presented in Fig. 4. This is consistent with the notion that the well depth scales with the magnitude of the polarization^{40,70}. Thus, the energy barrier is changed, already hinting at a variation in phase transition behavior when using different exchangecorrelation functionals.
Ultimately, we would like to understand the effects of exchange correlation functionals on dynamic phenomena such as phase transitions, domain wall motion and piezoelectric response; thus requiring the need to perform Monte Carlo or molecular dynamics simulations. However, as a first approximation it is possible to estimate phase transition temperatures (T_{c}) from the cubic phase to the tetragonal phase in these materials using Landau theory. In this regards, Grinberg and Rappe demonstrated that there exists a strong dependence of T_{c} on the local structures of Pb and Bibased solid solutions^{71,72}. Such dependence was expressed as a linear relationship between T_{c} and spontaneous polarization (P) in Landau theory as follows^{69}:
The constant γ of each crystal phase can be found by using the experimental spontaneous polarizations and temperatures. Thus, using such an approach, we can approximate T_{c} solely based on P from DFT calculations, as already summarized in Table 1. Of course, this approach cannot be used in a predictive sense as it requires experimental parameters to obtain the constant γ. Nevertheless, it emphasizes how small deviations in predictions of polarizations may be magnified in the prediction of other material behaviors. The estimated values of T_{c} from Equation (4) were determined over a large temperature range for different crystal phases of oxide perovskites, as shown in Fig. 5. Naturally, the phases with predicted P that are close to the experimental P yield the best agreement in T_{c} with experiment due to the nature of Equation (4). Again, the large variation in predicted temperatures is another indication that the exchangecorrelation functional needs to be carefully chosen in order to accurately describe the ferroelectric phase transition of perovskite oxides.
Conclusions
In conclusion, we studied how the choice of exchangecorrelation functional influences both the structural and ferroelectric properties of prototypical PbTiO_{3}, BaTiO_{3}, and KNbO_{3} perovskites. As expected, under and overestimations of lattice parameters and spontaneous polarizations were observed for LDA and PBE, respectively. In contrast, the opposite trend was seen in estimating the bulk modulus arising from the dependence of total energy on volume. Such variations in spontaneous polarizations and bulk moduli are a good (first) indication of exchange and correlation effects in predicting the responses in these materials. We found that a functional designed to describe sparse matter, vdWDFC09, gives the best agreement with experimental values for the structural properties. Similar performance was previously observed for a limited test of the vdWDFcx functional for the cubic and tetragonal phases of PTO. Both potentialwell depths and transition temperatures were also greatly affected by choice of functionals. Detailed analyses of the exchange enhancement factor reveal that the variations in properties are strongly tied to the behavior of enhancement factor observed in the small s region. The PBEsol and C09 exchange functionals reproduce the form of GEA, thereby being more appropriate functionals when studying dense solids. It is worth noting that other exchange functionals that are often paired with the vdWDF nonlocal correlation functional, including cx and optB86b, have similar forms in the small s region and may behave similarly for dense matter^{53,54}. Overall, the selection of exchangecorrelation functionals can induce nonnegligible variations in predicting macroscopic properties of ferroelectric perovskite oxides, stressing the importance of exchangecorrelation effects on such systems. In any event, these results provide benchmarks for the class of vdWDF functionals that help to emphasize the role that the exchange functional plays in defining structural (and perhaps dynamic) properties of materials. Nevertheless, such considerations should be taken into account in the design or parameterization of new empirical/phenomenological models for studying dynamic and temperature and pressuredependent properties of bulk complex oxides.
Additional Information
How to cite this article: Yuk, S. F. et al. Towards an accurate description of perovskite ferroelectrics: exchange and correlation effects. Sci. Rep. 7, 43482; doi: 10.1038/srep43482 (2017).
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Change history
03 May 2017
A correction has been published and is appended to both the HTML and PDF versions of this paper. The error has not been fixed in the paper.
03 May 2017
Scientific Reports 7: Article number: 43482; published online: 03 March 2017; updated: 03 May 2017 This Article contains errors. In the ‘Results and Discussion’ section, “…the exchange energy per particle in a uniform gas with KF = 3π2 n. For s < 2, F x(s) of vdWDFC09 matches PBEsol, which tends to the form of the gradient expansion approximation (GEA)67; where F_x(s) = 1 + \mu s2 with \mu = 0.
References
Jaffe, B., Roth, R. & Marzullo, S. Piezoelectric Properties of Lead ZirconateLead Titanate SolidSolution Ceramics. J. Appl. Phys. 25, 809–810 (1954).
Jaffe, B., Roth, R. & Marzullo, S. Properties of piezoelectric ceramics in the solidsolution series lead titanatelead zirconatelead oxide: tin oxide and lead titanatelead hafnate. J. Res. Nat. Bur. Stand. 55, 239–254 (1955).
Ouchi, H., Nagano, K. & Hayakawa, S. Piezoelectric properties of Pb(Mg1/3Nb2/3)O3—PbTiO3—PbZrO3 solid solution ceramics. J. Am. Ceram. Soc. 48, 630–635 (1965).
Ramesh, R. Thin Film Ferroelectric Materials and Devices (Springer, 2013).
Scott, J. F. Ferroelectric Memories (Springer, 2013).
Takenaka, T., Maruyama, K. & Sakata, K. (Bi1/2Na1/2)TiO3BaTiO3 system for leadfree piezoelectric ceramics. Jpn. J. Appl. Phys 30, 2236 (1991).
Guo, Y., Kakimoto, K. & Ohsato, H. (Na0.5K0.5)NbO3–LiTaO3 leadfree piezoelectric ceramics. Mater. Lett. 59, 241–244 (2005).
Takenaka, T. & Nagata, H. Current status and prospects of leadfree piezoelectric ceramics. J. Eur. Ceram. Soc. 25, 2693–2700 (2005).
Shrout, T. R. & Zhang, S. J. Leadfree piezoelectric ceramics: Alternatives for PZT? J. Electroceram. 19, 113–126 (2007).
Yejing, D., Xiaowen, Z. & Kepi, C. Morphotropic phase boundary and electrical properties of K1xNaxNbO3 leadfree ceramics. Appl. Phys. Lett. 94, 042905 (2009).
Zhong, W., Vanderbilt, D. & Rabe, K. M. Phase Transitions in BaTiO3 from First Principles. Phys. Rev. Lett. 73, 1861 (1994).
Zhong, W., Vanderbilt, D. & Rabe, K. M. Firstprinciples theory of ferroelectric phase transitions for perovskites: the case of BaTiO3 . Phys. Rev. B 52, 6301 (1995).
Waghmare, U. V. & Rabe, K. M. Ab initio statistical mechanics of the ferroelectric phase transition in PbTiO3 . Phys. Rev. B 55, 6161 (1997).
Vanderbilt, D. Firstprinciples based modelling of ferroelectrics. Curr. Opin. Solid State Mater. Sci. 2, 701–705 (1997).
Cohen, R. E. Theory of ferroelectrics: a vision for the next decade and beyond. J. Phys. Chem. Solids 61, 139–146 (2000).
Walizer, L., Lisenkov, S. & Bellaiche, L. Finitetemperature properties of (Ba, Sr)TiO3 systems from atomistic simulations. Phys. Rev. B 73, 144105 (2006).
BinOmran, S., Kornev, I. A. & Bellaiche, L. WangLandau Monte Carlo formalism applied to ferroelectrics. Phys. Rev. B 93, 014104 (2016).
Sepliarsky, M., Stachiotti, M. G. & Migoni, R. L. Ferroelectric soft mode and relaxation behavior in a moleculardynamics simulation of KNbO3 and KTaO3 . Phys. Rev. B 56, 566 (1997).
Sepliarsky, M., Asthagiri, A., Phillpot, S. R., Stachiotti, M. G. & Migoni, R. L. Atomiclevel simulation of ferroelectricity in oxide materials. Curr. Opin. Solid State Mater. Sci. 9, 107–113 (2005).
Sepliarsky, M., Phillpot, S. R., Stachiotti, M. G. & Migoni, R. L. Ferroelectric phase transitions and dynamical behavior in KNbO3/KTaO3 superlattices by moleculardynamics simulation. J. Appl. Phys. 91, 3165–3171 (2002).
Grinberg, I., Cooper, V. R. & Rappe, A. M. Relationship between local structure and phase transitions of a disordered solid solution. Nature 419, 909–911 (2002).
Cooper, V. R., Grinberg, I. & Rappe, A. M. In AIP Conference Proceedings. (eds Davies, P. K. & Singh, D. J. ) 220–230 (American Institute of Physics, 2003).
Shin, Y.H., Cooper, V. R., Grinberg, I. & Rappe, A. M. Development of a bondvalence moleculardynamics model for complex oxides. Phys. Rev. B 71, 054104 (2005).
Tinte, S., Stachiotti, M. G., Sepliarsky, M., Migoni, R. L. & Rodriguez, C. O. Atomistic modelling of BaTiO3 based on firstprinciples calculations. J. Phys. Condens. Matter 11, 9679 (1999).
Bersuker, I. B. Recent development of the vibronic theory of ferroelectricity. Ferroelectrics 164, 75–100 (1995).
Tinte, S., Íñiguez, J., Rabe, K. M. & Vanderbilt, D. Quantitative analysis of the firstprinciples effective Hamiltonian approach to ferroelectric perovskites. Phys. Rev. B 67, 064106 (2003).
Bersuker, I. B. The JahnTeller Effect (Cambridge University Press, 2006).
Lejaeghere, K., Van Speybroeck, V., Van Oost, G. & Cottenier, S. Error estimates for solidstate densityfunctional theory predictions: an overview by means of the groundstate elemental crystals. Crit. Rev. Solid State Mater. Sci. 39, 1–24 (2014).
Lejaeghere, K. et al. Reproducibility in density functional theory calculations of solids. Science 351, aad3000 (2016).
Tinte, S., Stachiotti, M. G., Rodriguez, C. O., Novikov, D. L. & Christensen, N. E. Applications of the generalized gradient approximation to ferroelectric perovskites. Phys. Rev. B 58, 11959 (1998).
KingSmith, R. D. & Vanderbilt, D. Firstprinciples investigation of ferroelectricity in perovskite compounds. Phys. Rev. B 49, 5828 (1994).
Cohen, R. E. & Krakauer, H. Lattice dynamics and origin of ferroelectricity in BaTiO3: Linearizedaugmentedplanewave totalenergy calculations. Phys. Rev. B 42, 6416 (1990).
Cohen, R. E. & Krakauer, H. Electronic structure studies of the differences in ferroelectric behavior of BaTiO3 and PbTiO3 . Ferroelectrics 136, 65–83 (1992).
Cohen, R. E. Origin of ferroelectricity in perovskite oxides. Nature 358, 136–138 (1992).
Singh, D. J. & Boyer, L. L. First principles analysis of vibrational modes in KNbO3 . Ferroelectrics 136, 95–103 (1992).
Singh, D. J. Local density and generalized gradient approximation studies of KNbO3 and BaTiO3 . Ferroelectrics 164, 143–152 (1995).
Rabe, K. M., Triscone, J.M. & Ahn, C. H. Modern Ferroelectrics. (Springer, 2007).
Wu, Z. & Cohen, R. E. More accurate generalized gradient approximation for solids. Phys. Rev. B 73, 235116 (2006).
Perdew, J. P. et al. Restoring the densitygradient expansion for exchange in solids and surfaces. Phys. Rev. Lett. 100, 136406 (2008).
Bilc, D. I. et al. Hybrid exchangecorrelation functional for accurate prediction of the electronic and structural properties of ferroelectric oxides. Phys. Rev. B 77, 165107 (2008).
Wahl, R., Vogtenhuber, D. & Kresse, G. SrTiO3 and BaTiO3 revisited using the projector augmented wave method: Performance of hybrid and semilocal functionals. Phys. Rev. B 78, 104116 (2008).
Rydberg, H. et al. Van der Waals density functional for layered structures. Phys. Rev. Lett. 91, 126402 (2003).
Dion, M., Rydberg, H., Schröder, E., Langreth, D. C. & Lundqvist, B. I. Van der Waals density functional for general geometries. Phys. Rev. Lett. 92, 246401 (2004).
Thonhauser, T. et al. Van der Waals density functional: Selfconsistent potential and the nature of the van der Waals bond. Phys. Rev. B 76, 125112 (2007).
Klimeš, J., Bowler, D. R. & Michaelides, A. Chemical accuracy for the van der Waals density functional. J. Phys. Condens. Matter 22, 022201 (2009).
RománPérez, G. & Soler, J. M. Efficient implementation of a van der Waals density functional: application to doublewall carbon nanotubes. Phys. Rev. Lett. 103, 096102 (2009).
Cooper, V. R. Van der Waals density functional: An appropriate exchange functional. Phys. Rev. B 81, 161104 (2010).
Lee, K., Murray, É. D., Kong, L., Lundqvist, B. I. & Langreth, D. C. Higheraccuracy van der Waals density functional. Phys. Rev. B 82, 081101 (2010).
Vydrov, O. A. & Van Voorhis, T. Nonlocal van der Waals density functional: The simpler the better. J. Chem. Phys. 133, 244103 (2010).
Klimeš, J., Bowler, D. R. & Michaelides, A. Van der Waals density functionals applied to solids. Phys. Rev. B 83, 195131 (2011).
Lee, K., Kolb, B., Thonhauser, T., Vanderbilt, D. & Langreth, D. C. Structure and energetics of a ferroelectric organic crystal of phenazine and chloranilic acid. Phys. Rev. B 86, 104102 (2012).
Berland, K. et al. van der Waals density functionals built upon the electrongas tradition: Facing the challenge of competing interactions. J. Chem. Phys. 140, 18A539 (2014).
Berland, K. et al. van der Waals forces in density functional theory: a review of the vdWDF method. Rep. Prog. Phys. 78, 066501 (2015).
Berland, K. & Hyldgaard, P. Exchange functional that tests the robustness of the plasmon description of the van der Waals density functional. Phys. Rev. B 89, 035412 (2014).
Gharaee, L., Erhart, P. & Hyldgaard, P. Finitetemperature properties of nonmagnetic transition metals: Comparison of the performance of constraintbased semi and nonlocal functionals. arXiv:1612.00425 (2016).
Giannozzi, P. et al. QUANTUM ESPRESSO: a modular and opensource software project for quantum simulations of materials. J. Phys. Condens. Matter 21, 395502 (2009).
Vanderbilt, D. Soft selfconsistent pseudopotentials in a generalized eigenvalue formalism. Phys. Rev. B 41, 7892 (1990).
Garrity, K. F., Bennett, J. W., Rabe, K. M. & Vanderbilt, D. Pseudopotentials for highthroughput DFT calculations. Comput. Mater. Sci. 81, 446–452 (2014).
Ceperley, D. M. & Alder, B. J. Ground state of the electron gas by a stochastic method. Phys. Rev. Lett. 45, 566 (1980).
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865 (1996).
KingSmith, R. D. & Vanderbilt, D. Theory of polarization of crystalline solids. Phys. Rev. B 47, 1651 (1993).
Birch, F. Finite elastic strain of cubic crystals. Phys. Rev. 71, 809 (1947).
Lines, M. E. & Glass, A. M. Principles and Applications of Ferroelectrics and Related Materials. (Oxford University Press, 1977).
Rabe, K. M., Dawber, M., Lichtensteiger, C., Ahn, C. H. & Triscone, J.M. Modern Physics of Ferroelectrics: Essential Background. (Springer, 2007).
Ogawa, T. In Ferroelectric Materials  Synthesis and Characterization (eds Barranco, A. P. ) 33–58 (InTech, 2015).
Grabowski, B., Hickel, T. & Neugebauer, J. Ab initio study of the thermodynamic properties of nonmagnetic elementary fcc metals: Exchangecorrelationrelated error bars and chemical trends. Phys. Rev. B 76, 024309 (2007).
Sham, L. J. Computational Methods in Band Theory. (Plenum, 1971).
Zhang, Y. & Yang, W. Comment on “Generalized gradient approximation made simple”. Phys. Rev. Lett. 80, 890 (1998).
Landau, L. D. On the theory of phase transitions. I. Zh. Eksp. Teor. Fiz. 11, 19 (1937).
Dall’Olio, S., Dovesi, R. & Resta, R. Spontaneous polarization as a Berry phase of the HartreeFock wave function: The case of KNbO3 . Phys. Rev. B 56, 10105 (1997).
Grinberg, I. & Rappe, A. M. Local structure and macroscopic properties in PbMg1∕ 3Nb2∕ 3O3 − PbTiO3 and PbZn1∕ 3Nb2∕ 3O3 − PbTiO3 solid solutions. Phys. Rev. B 70, 220101 (2004).
Grinberg, I. & Rappe, A. M. Nonmonotonic TC Trends in BiBased Ferroelectric Perovskite Solid Solutions. Phys. Rev. Lett. 98, 037603 (2007).
Mabud, S. A. & Glazer, A. M. Lattice parameters and birefringence in PbTiO3 single crystals. J. Appl. Crystallogr. 12, 49–53 (1979).
Sani, A., Hanfland, M. & Levy, D. The equation of state of PbTiO3 up to 37 GPa: a synchrotron xray powder diffraction study. J. Phys. Condens. Matter 14, 10601 (2002).
Shirane, G., Pepinsky, R. & Frazer, B. Xray and neutron diffraction study of ferroelectric PbTiO3 . Acta Crystallographica 9, 131–140 (1956).
Costa, S. C., Pizani, P. S., Rino, J. P. & Borges, D. S. Structural phase transition and dynamical properties of PbTiO3 simulated by molecular dynamics. J. Phys. Condens. Matter 17, 5771 (2005).
Haun, M. J., Furman, E., Jang, S. J., McKinstry, H. A. & Cross, L. E. Thermodynamic theory of PbTiO3 . J. Appl. Phys. 62, 3331–3338 (1987).
Jabarov, S. G. et al. Highpressure effect on the ferroelectricparaelectric transition in PbTiO3 . Phys. Solid State 53, 2300–2304 (2011).
Hellwege, K. H. & Hellwege, A. M. Ferroelectrics and Related Substances. (Springer, 1969).
Fischer, G. J., Wang, Z. & Karato, S.I. Elasticity of CaTiO3, SrTiO3 and BaTiO3 perovskites up to 3.0 GPa: the effect of crystallographic structure. Phys. Chem. Miner. 20, 97–103 (1993).
Kwei, G. H., Lawson, A. C., Billinge, S. J. L. & Cheong, S. W. Structures of the ferroelectric phases of barium titanate. J. Phys. Chem. 97, 2368–2377 (1993).
Wieder, H. H. Electrical behavior of barium titanatge single crystals at low temperatures. Phys. Rev. 99, 1161 (1955).
Chiang, Y.M., Kingery, W. D. & Birnie, D. P. Physical Ceramics: Principles for Ceramic Science and Engineering. (John Wiley & Sons, 1997).
Shirane, G., Danner, H. & Pepinsky, R. Neutron Diffraction Study of Orthorhombic BaTiO3 . Phys. Rev. 105, 856 (1957).
Hewat, A. W. Structure of rhombohedral ferroelectric barium titanate. Ferroelectrics 6, 215–218 (1973).
Hewat, A. W. Cubictetragonalorthorhombicrhombohedral ferroelectric transitions in perovskite potassium niobate: neutron powder profile refinement of the structures. J. Phys. C: Solid State Phys. 6, 2559 (1973).
Chervin, J. C., Itié, J. P., Gourdain, D. & Pruzan, P. Energy dispersive Xray diffraction study of KNbO3 up to 19 GPa at room temperature. Solid State Commun. 110, 247–251 (1999).
Kleemann, W., Schäfer, F. J. & Fontana, M. D. Crystal optical studies of spontaneous and precursor polarization in KNbO3 . Phys. Rev. B 30, 1148 (1984).
Shirane, G., Newnham, R. & Pepinsky, R. Dielectric Properties and Phase Transitions of NaNbO3 and (Na, K)NbO3 . Phys. Rev. 96, 581 (1954).
Gourdain, D. et al. Compression of KNbO3 up to 30 GPa: Transition sequence orthorhombic → tetragonal → cubic. Phys. Rev. B 65, 054104 (2002).
MichelCalendini, F. M., Peltier, M. & Micheron, F. Electron paramagnetic resonance of Fe^{3+} in orthorhombic KNbO3 . Solid State Commun. 33, 145–150 (1980).
Acknowledgements
S.F.Y., M.E., and V.R.C. are supported by the U.S. Department of Energy (DOE), Office of Science, Basic Energy Sciences, Materials Sciences and Engineering Division and the Office of Science Early Career Research Program. K.C.P. and S.M.N. are supported by the National Science Foundation (DMR 1309114). K.C.P. also acknowledges the internship through the Advanced Short Term Research Opportunity (ASTRO) program at Oak Ridge National Laboratory (ORNL), supported by the U.S. DOE, Office of Science, Basic Energy Sciences, Materials Sciences and Engineering Division and the Office of Science Early Career Research Program. Y.W.L. is sponsored by the U.S. DOE, Office of Advanced Scientific Computing Research. We gratefully acknowledge the computational resources provided by the National Energy Research Scientific Computing Center (NERSC), which is supported by the Office of Science of the U.S. DOE under Contract No. DEAC0205CH11231 and the Oak Ridge Leadership Computing Facility (OLCF), which is supported by the Office of Science of the U.S. DOE under Contract No. DEAC0500OR22725.
Author information
Authors and Affiliations
Contributions
V.R.C. conceived the original idea and S.F.Y. performed all the DFT calculations. S.F.Y., K.C.P., S.M.N., M.E., Y.W.L., and V.R.C. discussed and interpreted the results. S.F.Y. and V.R.C. led the writing and analysis efforts. S.F.Y. prepared the figures and table for the manuscript. All the authors reviewed and edited the manuscript.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Supplementary information
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Cite this article
Yuk, S., Pitike, K., Nakhmanson, S. et al. Towards an accurate description of perovskite ferroelectrics: exchange and correlation effects. Sci Rep 7, 43482 (2017). https://doi.org/10.1038/srep43482
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/srep43482
This article is cited by

Tunable ferroelectricity in oxygendeficient perovskites with Grenier structure
npj Computational Materials (2023)

Discovery of orthorhombic perovskite oxides with low thermal conductivity by firstprinciples calculations
Journal of Advanced Ceramics (2022)

A large modulation of electronphonon coupling and an emergent superconducting dome in doped strong ferroelectrics
Nature Communications (2021)

Landau–Devonshire thermodynamic potentials for displacive perovskite ferroelectrics from first principles
Journal of Materials Science (2019)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.